Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling


 Megan Harmon
 1 years ago
 Views:
Transcription
1 Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G , US E. rmanios Mechanical and erospace Engineering, University of Texas at rlington ox 98, 5 W. First Street, Woolf Hall 2, rlington, TX 7698, US SUMMRY Materialindependent necessary and sufficient conditions for hygrothermal curvature stability of laminated composite plates have been derived. Hygrothermally stable asymmetric solutions exist for laminates of five or more plies. These solutions have been optimized for maximum extensiontwist coupling, constructed, and tested to demonstrate improved coupling properties. Keywords: hygrothermal stability, extensiontwist coupling, elastic tailoring, classical lamination theory, design and testing ITROUCTIO Coupling of deformation modes can be used advantageously to elastically tailor the response of a composite structure. For example, extensiontwist coupling has applications ranging from wind turbine blades to tiltrotor aircraft. Other types of coupling include extensionbending, bendingtwist, and anticlastic coupling. Extensiontwist coupling is only achievable using asymmetric stacking sequences, which often produce hygrothermal instabilities, meaning that temperature or moisture changes cause bending or warping []. Past design methods involve obtaining the desired coupling properties then attempting to minimize hygrothermal effects [2]. The present work takes hygrothermal stability as the primary constraint then investigates the achievable elastic properties. The first established family of extensiontwistcoupled composites that retain hygrothermal stability was detailed by Winckler [3] and given by the stacking sequence [θ / (θ9) 2 / θ / θ / (9θ) 2 / θ]. () These Wincklertype laminates have been the industry standard since their introduction. review of their usage has been published previously [4]. It has been discovered, however, that this family does not contain all hygrothermally stable laminates. Further, it has also been found that Winckler s family does not maximize extensiontwist
2 coupling among laminates consisting of eight plies. This work first provides an overview of how hygrothermal stability is enforced as given in previous work [5]. Then it presents solutions and verification to maximized extensiontwist coupling. HYGROTHERML STILITY COITIOS s given in classical lamination theory [6] for a laminate made of specially orthotropic plies, the nonmechanical inplane forces and shears and outofplane moments and curvatures are related to the inplane strains and outofplane curvatures as M M M ( T, H) = where ij, ij, and ij are the inplane and coupling stiffness coefficients respectively and (_) (T,H) indicates nonmechanical quantities. Since hygrothermal stability can be defined has having the outofplane curvatures equal to zero for any change in temperature or moisture, this can be expressed as M M M ( T, H) = The nonmechanical inplane forces and shears and outofplane moments and curvatures for an nply laminate are given by M M M ( T, H) ( T, H) = T2 + T = T n k= 3 k cos2θ k cos2θ k sin 2 θk ε ε γ cos2θ n k cos2θ k = sin 2θ k ( 2k n ) where θ k is the angle of the k th ply, and T, T 2, and T 3 are solely functions of the material properties and temperature and moisture changes. Using (2), it can be proven that the necessary and sufficient conditions to ensure hygrothermal stability are either [5] ε ε γ κ κ κ (2) (3) (4)
3 (T,H) = (T,H) and (T,H) =M (T,H) =M (T,H) =M (T,H) = or (5a, b) ij =. Since the latter precludes extensiontwist coupling, the former condition is of primary interest to this work. It should be noted that when the conditions are replaced into (4), all the materialdependent parameters cancel, making the conditions material independent. symmetric stacking sequences that retain hygrothermal stability were found for families of laminates consisting of five or more plies. sensitivity analysis performed in previous work demonstrated that small perturbations in ply angle (typical of handlayup error) did not affect the outofplane stability of hygrothermally stable asymmetric laminates any more than it would affect symmetric laminates [5]. Finite element models and manufacturing of representative laminates verified the hygrothermal stability. OPTIMIZTIO OF EXTESIOTWIST COUPLIG s given in Classical Lamination Theory, the relationship between force and moment resultants and the midplane strains and curvatures are expressed as [6] = M M M ε ε γ + M κ κ M M κ ( T, H). (6) where all parameters are as given before. The midplane strains and curvatures may then be calculated as ε ε γ = κ κ κ M M M ε ε γ + κ κ κ ( T, H) For an axial load in the xdirection, the twist curvature can be expressed as ( T, H ) κ. (7) κ = +. (8)
4 non Therefore, is the parameter that governs extensiontwist coupling. dimensional performance parameter can then be expressed as η = ntle (9) where n is the number of plies, t is the lamina thickness, L is the specimen length, and E is the material modulus of elasticity along the fiber direction. Within the constraints of the hygrothermal stability conditions, an optimizer was used to identify stacking sequences for which extensiontwist coupling is maximized for each of five, six, eight, and ten plies. lso included for comparison is an optimized Wincklertype laminate. Extensiontwist coupling is material dependent, and a T3/976 graphite/epo material system was chosen; its properties are given in Table I. The optimizer uses sequential quadratic programming implementation in conjunction with the conditions in (5a) and random seed angles to arrive at an extremal value of the for a given number of plies. Table II lists the optimization results for each laminate along with the performance parameter. Table I. Material Properties of T3/976. E 5 GPa E 8.45 GPa G 4.3 GPa Ν.328 Thickness.52 mm Table II. Optimization results. Laminate Optimal Stacking Sequence (deg.) η 5ply [58.7/.4/45/78.6/3.3] ply [2.2/63.8/48.7/48.7/63.8/2.2] ply [2.5/72./57.9/29.6/29.6/57.9/72./2.5] 247 ply [.2/69./65.3/3.8/42./42./3.8/65.3/69./.2] 2453 Winckler [.5/ /.5/.5/ /.5] 28 EXTESIOTWIST EXPERIMETL VERIFICTIO ll five laminates in Table II were constructed from a preimpregnated T3/976 graphite/epo material system with properties given in Table I. Each ply was hand cut, laid up in a flat aluminium mold, and cured in an autoclave with a cure cycle given in Figure. Cured laminates were confirmed to be hygrothermally stable by fixing three corners and measuring the displacement of the fourth corner. This value was shown to be the same for both antisymmetric layups and their symmetric counterparts. For example, [2.2/63.8/48.7/48.7/63.8/2.2] is the symmetric counterpart of the sixply extensiontwistoptimized laminate. Since symmetric layups are known to be hygrothermally stable, warping in these laminates are a quantitative measure of manufacturing imperfections.
5 Figure. Curing Cycle for Graphite/Epo Material. Each laminate was cut into five specimens of approximately 2.54 cm by 7.78 cm (. by 7. ) and tested in an Instron 8874 biaxial tensiontorsion machine. Specimens were taken from the center of each laminate to reduce the edge effects. Errors in the cutting process caused one specimen to be discarded from each of the six and tenply laminates. fter each specimen was installed in the machine, the tip twist under no axial load, termed pretwist, was recorded. Then, a load increment was applied, and, because of the specimens low torsion stiffness, the tip was rotated manually until the machine torque indicated a zero value. The load was applied in increments of 445 ( lb) up to 25 (5 lb). Figure 2 shows a specimen undergoing testing. The recorded data are plotted in Figures 3 through 6 for the sixply, eightply, tenply, and Wincklertype laminate, respectively. The test data from each specimen is referred to in each figure as Experimental, Experimental 2, etc. Initial pretwist values resulting from imperfections in the manufacturing process account for nonzero twists at no loading. lso included on each plot is a nonlinear model prediction for extensiontwist developed by rmanios et al [7] expressed as 4 b + F = 3 a ϕ b2 ol 2 [ b ( ϕ + ϕ )] 4 L + bϕ 2 3 ol ol ϕ L () where F a is axial force, φ ol is the tip pretwist angle, φ L is the tip twist angle, and b b 4 are functions of the inplane, ij, coupling, ij, and bending, ij, [7] stiffness coefficients, respectively. The nonlinear model is only valid for antisymmetric stacking sequences, and therefore the fiveply laminate is not included in these results. There is good correlation between the experimental data and the model for all laminates.
6 Figures 7 and 8 plot averaged test data along with maximum and minimum range overlaid with the nonlinear model for all four laminates to illustrate the improved coupling properties of the new classes. The abscissa in Figure 7 is the axial force and shows that all new laminates surpass the Wincklertype laminate. Further, laminates with fewer plies have more coupling; this can be explained when considering the lower torsional stiffness of a thinner laminate. Table III gives the percent increase in coupling of each laminate over the Wincklertype laminate. The abscissa in Figure 8 is axial stress, determined by dividing the axial force by the crosssectional area of the laminate. gain, all new laminates outperform the Wincklertype laminate; however, the tenply laminate outperforms the eightply laminate. Table IV gives the percent increase in coupling of each laminate over the Wincklertype laminate for this case. Monte Carlo simulation was performed to analyze the robustness of extensiontwist coupling to small errors in ply angle typically found in handlayup manufacturing. The sixply optimized extensiontwist laminate was chosen as representative, and the ply angles were varied in a uniform distribution on the interval θ k ±2, typical of errors seen in handlayup manufacturing. set of 6 samples were taken, was calculated, and the error was calculated. Figure 9 plots the distribution of the error for all samples. The reduction in coupling of perturbed laminates was bounded by % of its original coupling ability. Figure 2. Specimen Undergoing Testing in an Instron iaxial TensionTorsion Machine.
7 Twist (degrees) 5 5 onlinear Experimental Experimental 2 Experimental 3 Experimental Force () Figure 3. Maximized ExtensionTwist Coupling of SixPly Laminate 4 Twist (degrees) onlinear Experimental Experimental 2 Experimental 3 Experimental 4 Experimental Force () Figure 4. Maximized ExtensionTwist Coupling of EightPly Laminate
8 8 Twist (degrees) onlinear Experimental Experimental 2 Experimental 3 Experimental 4 Experimental Force () Figure 5. Maximized ExtensionTwist Coupling of TenPly Laminate 8 4 Twist (degrees) onlinear 2 Experimental Experimental 2 Experimental 3 Experimental Force () Figure 6. Maximized ExtensionTwist Coupling of a Winckler Laminate
9 Twist Rate ( o /m) SixPly SixPly EightPly EightPly TenPly TenPly Winckler Winckler Force () Figure 7. Comparison of veraged ExtensionTwist Coupling for ll Laminates Twist Rate ( o /m) SixPly SixPly EightPly EightPly TenPly TenPly Winckler Winckler Stress (MPa) x 7 Figure 8. Comparison of veraged ExtensionTwist Coupling for ll Laminates
10 Table III. Improvement over WincklerType Laminates when Compared at the Same Force. xial Load (lb) 6ply 8ply ply 9.% 28.9% 6.3% % 3.%.4% 3 76.% 29.7% 7.2% % 3.% 2.6% % 3.2% 25.9% verage 82.6% 29.8%.7% Table IV. Improvement over WincklerType Laminates when Compared at the Same Stress. xial Stress (MPa) 6ply 8ply ply 52.4%.% 2.8% %.% 28.8% % 2.6% 29.9% 4 4.% 2.2% 3.7% % 29.% 2.7% verage 46.5% 23.2%.2% 2 x Counts Error from maximum Figure 9. Histogram of Error ased on Uniform Plyngle Perturbation
11 COCLUSIOS ecessary and sufficient conditions for hygrothermal stability have been derived, with an overview provided in this work. The conditions can be summarized as either having the coupling stiffness matrix equal to zero or the outofplane moments and inplane shear force equal to zero along with both inplane axial forces equal to each other. From within these conditions, stacking sequences that maximize extensiontwist coupling have been found for laminates consisting of five, six, eight, and ten plies. The six, eight, and tenply laminates have been constructed and tested to demonstrate their improved coupling properties over the previouslyknown Wincklertype laminates. When compared at the same axial force level, the best laminate, the sixply laminate, outperforms the Wincklertype laminate by an average of 83%. When compared at the same stress level, the improvement averages 46%. n investigation of the benefits of the hygrothermal stability conditions on other types of couplings is underway. CKOWLEGEMETS The authors gratefully acknowledge the support given by the ational efense Science and Engineering Graduate Fellowship and the University of Texas System STRS Program. References. Hyer, M.W., Some Observations on the Curved Shape of Thin Unsymmetric Laminates, Journal of Composite Materials, Vol. 5, (2), 98, pp rmanios, E.., Hooke,., Kamat, M., Palmer,. and Li, J., esign and Testing of Composite Laminates with Optimum Extensiontwist Coupling, Composite Materials: Testing and esign, edited by E.T. Camponeschi Jr, Vol., merican Society for Testing and Materials, Philadelphia, P, 993, pp Winckler, S. I., Hygrothermally Curvature Stable Laminates with Tensiontorsion Coupling, Journal of the merican Helicopter Society, Vol. 3, (7), Haynes, R., Carey, R., and rmanios, E.., ew Class of Hygrothermally Stable Laminates with Extensiontwist Coupling, in Proceedings of the HS 65 th nnual Forum, Grapevine, TX, US, May, Cross, R.J., Haynes, R.., and rmanios, E.., Families of Hygrothermally Stable symmetric Laminated Composites, Journal of Composite Materials, Vol. 42, (7), 28, pp Jones, R. M., Mechanics of Composite Materials, 2nd Ed., Taylor & Francis, Philadelphia, P, 999, pp rmanios, E.., Makeev,., and Hooke,., Finiteisplacement nalysis of Laminated Composite Strips with ExtensionTwist Coupling, Journal of erospace Engineering, Vol. 9, (3), 996.
Bending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationMODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE
8th International DAAAM Baltic Conference INDUSTRIAL ENGINEERING 1921 April 2012, Tallinn, Estonia MODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE Pabut, O.; Allikas, G.; Herranen,
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationANALYSIS OF TAPERED LAMINATED COMPOSITE TUBES UNDER TENSION AND TORSION CHETHANA SHANKARA RAO. Presented to the Faculty of the Graduate School of
ANALYSIS OF TAPERED LAMINATED COMPOSITE TUBES UNDER TENSION AND TORSION by CHETHANA SHANKARA RAO Presented to the Faculty of the Graduate School of The University of Teas at Arlington in Partial Fulfillment
More informationQuestion 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H
Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The
More information11 Locate the centroid of the plane area shown. 12 Determine the location of centroid of the composite area shown.
Chapter 1 Review of Mechanics of Materials 11 Locate the centroid of the plane area shown 650 mm 1000 mm 650 x 1 Determine the location of centroid of the composite area shown. 00 150 mm radius 00 mm
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationBilinear Quadrilateral (Q4): CQUAD4 in GENESIS
Bilinear Quadrilateral (Q4): CQUAD4 in GENESIS The Q4 element has four nodes and eight nodal dof. The shape can be any quadrilateral; we ll concentrate on a rectangle now. The displacement field in terms
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationOutline. Organization. Stresses in Beams
Stresses in Beams B the end of this lesson, ou should be able to: Calculate the maimum stress in a beam undergoing a bending moment 1 Outline Curvature Normal Strain Normal Stress Neutral is Moment of
More informationAgnieszka Bondyra, Pawe Gotowicki
Journal of KONES Powertrain and Transport, Vol. 17, No. 1 21 INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationCIVL222 STRENGTH OF MATERIALS. Chapter 6. Torsion
CIVL222 STRENGTH OF MATERIALS Chapter 6 Torsion Definition Torque is a moment that tends to twist a member about its longitudinal axis. Slender members subjected to a twisting load are said to be in torsion.
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationA copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. (2015) On tapered warpfree laminates with singleply terminations. Composites Part A: Applied Science and Manufacturing, 72, pp. 127138. Copyright 2015 Elsevier Ltd. A copy can be downloaded
More informationRELIABILITYBASED DESIGN AND OPTIMIZATION OF SELFTWISTING COMPOSITE MARINE ROTORS
Proceedings of the ASME 28th International Conference on Ocean, Offshore and Arctic Engineering OMAE29 May 3June 5, 29, Honolulu, Hawaii OMAE29867 RELIABILITYBASED DESIGN AND OPTIMIZATION OF SELFTWISTING
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationExternal Work. When a force F undergoes a displacement dx in the same direction i as the force, the work done is
Structure Analysis I Chapter 9 Deflection Energy Method External Work Energy Method When a force F undergoes a displacement dx in the same direction i as the force, the work done is du e = F dx If the
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationThe stiffness tailoring of megawatt wind turbine
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The stiffness tailoring of megawatt wind turbine To cite this article: Z M Li et al 2013 IOP Conf. Ser.: Mater. Sci. Eng. 52 052008
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationSTRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS
STRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS By Joseph F. Murphy 1 ABSTRACT: Four large glulam beams with notches on the tension side were tested for strength and stiffness. Using either bending
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationSTRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK Md. S. Uddin 1*, E. V. Morozov 1 and K. Shankar 1 1 School of Engineering and Information
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More information6.1 Formulation of the basic equations of torsion of prismatic bars (St. Venant) Figure 6.1: Torsion of a prismatic bar
Module 6 Torsion Learning Objectives 6.1 Formulation of the basic equations of torsion of prismatic bars (St. Venant) Readings: Sadd 9.3, Timoshenko Chapter 11 e e 1 e 3 Figure 6.1: Torsion of a prismatic
More informationLinear plate bending and laminate theory
Linear plate bending and laminate theor 4M: Design Tools Eindhoven Universit of Technolog Linear plate bending A plate is a bod of which the material is located in a small region around a surface in the
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 4 Pure Bending
EA 3702 echanics & aterials Science (echanics of aterials) Chapter 4 Pure Bending Pure Bending Ch 2 Aial Loading & Parallel Loading: uniform normal stress and shearing stress distribution Ch 3 Torsion:
More informationIdentification of structural nonlinearities due to large deflections on a 5MW wind turbine blade
Identification of structural nonlinearities due to large deflections on a 5MW wind turbine blade V. A. Riziotis and S. G. Voutsinas National Technical University of Athens 9 Heroon Polytechniou str.,
More informationComparison between the basic least squares and the Bayesian approach for elastic constants identification
Comparison between the basic least squares and the ayesian approach for elastic constants identification C Gogu 1,,3, R Haftka, R Le Riche 1, J Molimard 1, Vautrin 1, Sankar 1 Ecole des Mines de Saint
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationDEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS
DEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS THE INFLUENCE OF THE FORM OF A WOODEN BEAM ON ITS STIFFNESS AND STRENGTHI (REPRINT FROM NATIONAL ADVISORY COMMITTEE FOR AERONAUTICS REPORT
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationBeam Models. Wenbin Yu Utah State University, Logan, Utah April 13, 2012
Beam Models Wenbin Yu Utah State University, Logan, Utah 8434130 April 13, 01 1 Introduction If a structure has one of its dimensions much larger than the other two, such as slender wings, rotor blades,
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationOptimum Fiber Distribution in Singlewall Corrugated Fiberboard
United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPL 348 1979 Optimum Fiber Distribution in Singlewall Corrugated Fiberboard Abstract Determining optimum
More informationPlease review the following statement: I certify that I have not given unauthorized aid nor have I received aid in the completion of this exam.
Group Number: Please review the following statement: I certify that I have not given unauthorized aid nor have I received aid in the completion of this exam. Signature: INSTRUCTIONS Begin each problem
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationKirchhoff Plates: Field Equations
20 Kirchhoff Plates: Field Equations AFEM Ch 20 Slide 1 Plate Structures A plate is a three dimensional bod characterized b Thinness: one of the plate dimensions, the thickness, is much smaller than the
More informationTorsion Stresses in Tubes and Rods
Torsion Stresses in Tubes and Rods This initial analysis is valid only for a restricted range of problem for which the assumptions are: Rod is initially straight. Rod twists without bending. Material is
More informationSample Problems for Exam II
Sample Problems for Exam 1. Te saft below as lengt L, Torsional stiffness GJ and torque T is applied at point C, wic is at a distance of 0.6L from te left (point ). Use Castigliano teorem to Calculate
More informationValidation of the Resonalyser method: an inverse method for material identification
Validation of the Resonalyser method: an inverse method for material identification T. Lauwagie, H. Sol,. Roebben 3, W. Heylen and Y. Shi Katholieke Universiteit Leuven (KUL) Department of Mechanical ngineering
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationReview of Strain Energy Methods and Introduction to Stiffness Matrix Methods of Structural Analysis
uke University epartment of Civil and Environmental Engineering CEE 42L. Matrix Structural Analysis Henri P. Gavin Fall, 22 Review of Strain Energy Methods and Introduction to Stiffness Matrix Methods
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More information4. SHAFTS. A shaft is an element used to transmit power and torque, and it can support
4. SHAFTS A shaft is an element used to transmit power and torque, and it can support reverse bending (fatigue). Most shafts have circular cross sections, either solid or tubular. The difference between
More informationA review on the mechanical behaviour of curvilinear fibre composite laminated panels
A review on the mechanical behaviour of curvilinear fibre composite laminated panels Pedro Ribeiro, Hamed Ahavan IDMEC/DEMec, Faculdade de Engenharia, Universidade do Porto Porto, Portugal Andrzej Teter,
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationDeflections and Strains in Cracked Shafts Due to Rotating Loads: A Numerical and Experimental Analysis
International Journal of Rotating Machinery, 9: 303 311, 2003 Copyright c Taylor & Francis Inc. ISSN: 1023621X DOI: 10.1080/10236210390147416 Deflections and Strains in Cracked Shafts Due to Rotating
More informationSTRESSEDSKIN PANEL DEFLECTIONS AND STRESSES USDA FOREST SERVICE RESEARCH PAPER
STRESSEDSKIN PANEL DEFLECTIONS AND STRESSES USDA FOREST SERVICE RESEARCH PAPER FPL 251 1975 U. S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WISCONSIN ABSTRACT This paper
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationModule 4 : Deflection of Structures Lecture 4 : Strain Energy Method
Module 4 : Deflection of Structures Lecture 4 : Strain Energy Method Objectives In this course you will learn the following Deflection by strain energy method. Evaluation of strain energy in member under
More informationFlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal Unbraced Lengths
Proceedings of the Annual Stability Conference Structural Stability Research Council San Antonio, Texas, March 2124, 2017 FlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal
More informationDate Submitted: 1/8/13 Section #4: T Instructor: Morgan DeLuca. Abstract
Lab Report #2: Poisson s Ratio Name: Sarah Brown Date Submitted: 1/8/13 Section #4: T 1012 Instructor: Morgan DeLuca Group Members: 1. Maura Chmielowiec 2. Travis Newberry 3. Thomas Cannon Title: Poisson
More informationMulti physics design and optimization of flexible matrix composite (FMC) driveshafts
Research Collection Master Thesis Multi physics design and optimization of flexible matrix composite (FMC) driveshafts Author(s): Roos, Christoph Publication Date: 2010 Permanent Link: https://doi.org/10.3929/ethza010076645
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationCurvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment. P. Krulevitch G. C. Johnson
UCRLJC30440 PREPRINT Curvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment P. Krulevitch G. C. Johnson This paper was prepared for submittal to the Materials Research Society Spring
More informationBME 207 Introduction to Biomechanics Spring 2017
April 7, 2017 UNIVERSITY OF RHODE ISAND Department of Electrical, Computer and Biomedical Engineering BE 207 Introduction to Biomechanics Spring 2017 Homework 7 Problem 14.3 in the textbook. In addition
More informationUnified Quiz M4 May 7, 2008 M  PORTION
9:0010: 00 (last four digits) 32141 Unified Quiz M4 May 7, 2008 M  PORTION Put the last four digits of your MIT ID # on each page of the exam. Read all questions carefully. Do all work on that question
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationShear of Thin Walled Beams. Introduction
Introduction Apart from bending, shear is another potential structural failure mode of beams in aircraft For thinwalled beams subjected to shear, beam theory is based on assumptions applicable only to
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More information